#------------------------------------------------------------------------------
#$Date: 2016-02-14 06:40:26 +0200 (Sun, 14 Feb 2016) $
#$Revision: 176432 $
#$URL: svn://www.crystallography.net/cod/cif/7/20/97/7209788.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7209788
loop_
_publ_author_name
'Zhang, Zhe'
'Yang, Jin'
'Liu, Ying-Ying'
'Ma, Jian-Fang'
_publ_section_title
;
 Five polyoxometalate-based inorganic--organic hybrid compounds
 constructed by a multidentate N-donor ligand: syntheses, structures,
 electrochemistry, and photocatalysis properties
;
_journal_issue                   19
_journal_name_full               CrystEngComm
_journal_page_first              3843
_journal_paper_doi               10.1039/c3ce40210j
_journal_volume                  15
_journal_year                    2013
_chemical_formula_moiety         'C24 H40 Co2 Mo8 N18 O34'
_chemical_formula_sum            'C24 H40 Co2 Mo8 N18 O34'
_chemical_formula_weight         2010.12
_chemical_name_systematic
;
?
;
_space_group_IT_number           2
_symmetry_cell_setting           triclinic
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                87.135(6)
_cell_angle_beta                 72.428(6)
_cell_angle_gamma                66.412(7)
_cell_formula_units_Z            1
_cell_length_a                   10.5490(7)
_cell_length_b                   10.8420(7)
_cell_length_c                   13.8000(9)
_cell_measurement_reflns_used    3029
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      29.1058
_cell_measurement_theta_min      3.1008
_cell_volume                     1374.43(18)
_computing_cell_refinement       CrysAlis
_computing_data_collection       'CrysAlis (Oxford Diffraction, 2006)'
_computing_data_reduction        CrysAlis
_computing_structure_refinement  'SHELXS-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1997)'
_diffrn_ambient_temperature      293(2)
_diffrn_detector_area_resol_mean 10.0
_diffrn_measured_fraction_theta_full 0.996
_diffrn_measured_fraction_theta_max 0.996
_diffrn_measurement_device_type  'Oxford Diffraction Gemini R Ultra'
_diffrn_measurement_method       'ω scan'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71069
_diffrn_reflns_av_R_equivalents  0.0337
_diffrn_reflns_av_sigmaI/netI    0.0582
_diffrn_reflns_limit_h_max       12
_diffrn_reflns_limit_h_min       -12
_diffrn_reflns_limit_k_max       13
_diffrn_reflns_limit_k_min       -12
_diffrn_reflns_limit_l_max       14
_diffrn_reflns_limit_l_min       -16
_diffrn_reflns_number            8753
_diffrn_reflns_theta_full        25.34
_diffrn_reflns_theta_max         25.34
_diffrn_reflns_theta_min         3.11
_exptl_absorpt_coefficient_mu    2.458
_exptl_absorpt_correction_T_max  0.7094
_exptl_absorpt_correction_T_min  0.6264
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
CrysAlis (Oxford Diffraction, 2006)
;
_exptl_crystal_colour            pink
_exptl_crystal_density_diffrn    2.429
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       block
_exptl_crystal_F_000             972
_exptl_crystal_size_max          0.21
_exptl_crystal_size_mid          0.17
_exptl_crystal_size_min          0.15
_refine_diff_density_max         0.743
_refine_diff_density_min         -0.838
_refine_diff_density_rms         0.137
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.026
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     424
_refine_ls_number_reflns         5015
_refine_ls_number_restraints     54
_refine_ls_restrained_S_all      1.041
_refine_ls_R_factor_all          0.0572
_refine_ls_R_factor_gt           0.0379
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0346P)²+0.8816P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0823
_refine_ls_wR_factor_ref         0.0908
_reflns_number_gt                3838
_reflns_number_total             5015
_reflns_threshold_expression     >2σ(I)
_cod_data_source_file            c3ce40210j.txt
_cod_data_source_block           Compound-4
_cod_depositor_comments
;
The following automatic conversions were performed:

'_symmetry_cell_setting' value 'Triclinic' changed to 'triclinic'
according to /home/saulius/struct/CIF-dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 1891 2012-01-12 08:04:46Z andrius 
;
_cod_original_sg_symbol_Hall     '-P 1 '
_cod_original_sg_symbol_H-M      p-1
_cod_database_code               7209788
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, -z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
Co1 Co 0.49638(9) 0.68178(8) -0.15793(6) 0.0210(2) Uani 1 1 d .
Mo1 Mo 0.02505(5) 0.50140(5) -0.13399(3) 0.01696(13) Uani 1 1 d .
Mo2 Mo 0.32442(6) 0.20912(5) -0.13127(4) 0.02374(15) Uani 1 1 d .
Mo3 Mo 0.01004(6) 0.22915(5) 0.01750(4) 0.02171(14) Uani 1 1 d .
Mo4 Mo 0.28144(5) 0.48368(5) -0.01517(4) 0.01725(13) Uani 1 1 d .
C1 C 0.5934(8) 1.4149(7) -0.2947(5) 0.0419(18) Uani 1 1 d .
H1 H 0.5014 1.4136 -0.2742 0.050 Uiso 1 1 calc R
C2 C 0.7675(11) 1.4712(10) -0.3167(8) 0.075(2) Uani 1 1 d U
C3 C 0.7124(7) 1.2172(6) -0.4270(5) 0.0290(15) Uani 1 1 d .
H3A H 0.6820 1.2548 -0.4855 0.035 Uiso 1 1 calc R
H3B H 0.6453 1.1792 -0.3881 0.035 Uiso 1 1 calc R
C4 C 0.8625(6) 1.1068(5) -0.4634(4) 0.0154(12) Uani 1 1 d .
C5 C 0.9095(6) 0.9998(6) -0.4022(4) 0.0186(12) Uani 1 1 d .
C6 C 1.0443(6) 0.8946(5) -0.4395(4) 0.0183(12) Uani 1 1 d .
C7 C 1.0920(7) 0.7775(6) -0.3746(5) 0.0274(14) Uani 1 1 d .
H7A H 1.0068 0.7712 -0.3262 0.033 Uiso 1 1 calc R
H7B H 1.1459 0.6939 -0.4181 0.033 Uiso 1 1 calc R
C8 C 1.2552(9) 0.8930(7) -0.2340(6) 0.0450(19) Uani 1 1 d .
H8 H 1.2657 0.9597 -0.2014 0.054 Uiso 1 1 calc R
C9 C 1.2889(7) 0.7010(6) -0.2886(5) 0.0318(15) Uani 1 1 d .
H9 H 1.3230 0.6085 -0.3037 0.038 Uiso 1 1 calc R
C10 C 0.8106(7) 1.0016(6) -0.2958(4) 0.0267(14) Uani 1 1 d .
H10A H 0.8677 0.9735 -0.2490 0.032 Uiso 1 1 calc R
H10B H 0.7387 1.0930 -0.2733 0.032 Uiso 1 1 calc R
C11 C 0.6779(7) 0.8552(6) -0.2135(4) 0.0261(14) Uani 1 1 d .
H11 H 0.6826 0.8614 -0.1478 0.031 Uiso 1 1 calc R
C12 C 0.6329(9) 0.8104(8) -0.3415(5) 0.044(2) Uani 1 1 d .
H12 H 0.5965 0.7757 -0.3818 0.053 Uiso 1 1 calc R
N1 N 0.6128(6) 0.7900(5) -0.2423(4) 0.0266(12) Uani 1 1 d .
N2 N 0.7368(6) 0.9121(5) -0.2935(4) 0.0252(12) Uani 1 1 d .
N3 N 0.7078(7) 0.8832(7) -0.3768(4) 0.0459(17) Uani 1 1 d .
N4 N 1.3381(6) 0.7571(5) -0.2343(4) 0.0249(12) Uani 1 1 d .
N5 N 1.1836(6) 0.7949(5) -0.3191(4) 0.0283(12) Uani 1 1 d .
N6 N 1.1609(8) 0.9199(5) -0.2836(5) 0.0470(17) Uani 1 1 d .
N7 N 0.6227(7) 1.5051(5) -0.2581(4) 0.0367(13) Uani 1 1 d U
N8 N 0.7050(6) 1.3260(6) -0.3631(4) 0.0374(14) Uani 1 1 d .
N9 N 0.8201(10) 1.3681(9) -0.3869(7) 0.060(2) Uani 0.80 1 d PU
N9A N 0.822(4) 1.312(3) -0.331(2) 0.049(8) Uani 0.20 1 d PU
O1 O -0.1033(5) 0.1584(4) 0.0090(3) 0.0344(11) Uani 1 1 d .
O2 O -0.1291(4) 0.3969(4) 0.1077(3) 0.0183(8) Uani 1 1 d .
O3 O 0.0902(5) 0.1449(4) 0.1043(3) 0.0362(11) Uani 1 1 d .
O4 O -0.0556(5) 0.5963(4) -0.2164(3) 0.0281(10) Uani 1 1 d .
O5 O -0.1236(4) 0.6156(4) 0.0051(3) 0.0179(8) Uani 1 1 d .
O6 O 0.4367(5) 0.1257(4) -0.2455(4) 0.0414(12) Uani 1 1 d .
O8 O 0.3775(4) 0.3598(4) -0.1301(3) 0.0236(9) Uani 1 1 d .
O9 O 0.3548(4) 0.3907(4) 0.0738(3) 0.0219(9) Uani 1 1 d .
O10 O 0.3697(4) 0.5883(4) -0.0536(3) 0.0252(10) Uani 1 1 d .
O11 O 0.0936(4) 0.6020(4) 0.0822(3) 0.0194(9) Uani 1 1 d .
O12 O 0.1772(5) 0.3687(4) -0.2095(3) 0.0255(9) Uani 1 1 d .
O13 O 0.1645(5) 0.1591(4) -0.1060(3) 0.0271(10) Uani 1 1 d .
O14 O 0.4023(5) 0.1207(4) -0.0438(4) 0.0388(12) Uani 1 1 d .
O1W O 0.3776(5) 0.8460(4) -0.0450(3) 0.0330(11) Uani 1 1 d .
O2W O 0.433(2) 0.157(2) -0.4508(14) 0.157(7) Uani 0.50 1 d PU
O3W O 0.149(2) 0.1970(19) -0.3949(12) 0.184(7) Uani 0.70 1 d P
O4W O 0.339(3) 0.406(3) -0.4227(16) 0.130(10) Uani 0.40 1 d P
O4WA O 0.394(2) 0.451(2) -0.4646(15) 0.154(7) Uani 0.60 1 d PU
O5W O -0.074(3) 0.201(3) -0.236(2) 0.112(9) Uani 0.30 1 d PU
O6W O 0.097(3) 0.441(3) -0.4468(17) 0.217(12) Uani 0.50 1 d P
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Co Co 0.3494 0.9721 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
N1 Co1 N4 92.11(19) . 1_455
N1 Co1 O9 90.02(17) . 2_665
N4 Co1 O9 176.81(18) 1_455 2_665
N1 Co1 N7 93.5(2) . 1_545
N4 Co1 N7 93.9(2) 1_455 1_545
O9 Co1 N7 88.38(19) 2_665 1_545
N1 Co1 O1W 89.62(18) . .
N4 Co1 O1W 91.43(19) 1_455 .
O9 Co1 O1W 86.20(16) 2_665 .
N7 Co1 O1W 173.76(19) 1_545 .
N1 Co1 O10 172.30(18) . .
N4 Co1 O10 90.76(17) 1_455 .
O9 Co1 O10 86.84(15) 2_665 .
N7 Co1 O10 93.45(18) 1_545 .
O1W Co1 O10 83.16(16) . .
O4 Mo1 O12 105.15(19) . .
O4 Mo1 O2 101.39(17) . 2_565
O12 Mo1 O2 96.41(17) . 2_565
O4 Mo1 O11 102.03(17) . 2_565
O12 Mo1 O11 96.63(17) . 2_565
O2 Mo1 O11 149.10(15) 2_565 2_565
O4 Mo1 O5 99.07(18) . .
O12 Mo1 O5 155.77(16) . .
O2 Mo1 O5 79.13(14) 2_565 .
O11 Mo1 O5 77.51(14) 2_565 .
O4 Mo1 O5 174.49(18) . 2_565
O12 Mo1 O5 80.27(16) . 2_565
O2 Mo1 O5 76.74(13) 2_565 2_565
O11 Mo1 O5 78.03(14) 2_565 2_565
O5 Mo1 O5 75.52(15) . 2_565
O4 Mo1 Mo4 91.39(14) . 2_565
O12 Mo1 Mo4 132.10(12) . 2_565
O2 Mo1 Mo4 124.39(11) 2_565 2_565
O11 Mo1 Mo4 35.51(11) 2_565 2_565
O5 Mo1 Mo4 45.32(9) . 2_565
O5 Mo1 Mo4 85.54(9) 2_565 2_565
O6 Mo2 O14 105.1(2) . .
O6 Mo2 O13 103.5(2) . .
O14 Mo2 O13 99.8(2) . .
O6 Mo2 O8 101.62(19) . .
O14 Mo2 O8 98.03(19) . .
O13 Mo2 O8 144.02(17) . .
O6 Mo2 O12 90.81(19) . .
O14 Mo2 O12 163.9(2) . .
O13 Mo2 O12 77.82(16) . .
O8 Mo2 O12 76.44(16) . .
O6 Mo2 O5 160.15(19) . 2_565
O14 Mo2 O5 94.55(19) . 2_565
O13 Mo2 O5 75.06(14) . 2_565
O8 Mo2 O5 72.60(14) . 2_565
O12 Mo2 O5 69.44(13) . 2_565
O1 Mo3 O3 105.8(2) . .
O1 Mo3 O13 102.2(2) . .
O3 Mo3 O13 101.4(2) . .
O1 Mo3 O2 101.27(19) . .
O3 Mo3 O2 97.10(19) . .
O13 Mo3 O2 144.75(15) . .
O1 Mo3 O11 88.52(17) . 2_565
O3 Mo3 O11 163.15(17) . 2_565
O13 Mo3 O11 83.79(16) . 2_565
O2 Mo3 O11 70.85(14) . 2_565
O1 Mo3 O5 159.73(17) . 2_565
O3 Mo3 O5 94.20(17) . 2_565
O13 Mo3 O5 76.75(14) . 2_565
O2 Mo3 O5 72.18(13) . 2_565
O11 Mo3 O5 71.21(12) 2_565 2_565
O10 Mo4 O9 105.45(18) . .
O10 Mo4 O8 97.91(18) . .
O9 Mo4 O8 101.33(18) . .
O10 Mo4 O11 103.49(17) . .
O9 Mo4 O11 96.61(17) . .
O8 Mo4 O11 147.20(16) . .
O10 Mo4 O5 159.42(16) . 2_565
O9 Mo4 O5 95.13(15) . 2_565
O8 Mo4 O5 77.69(15) . 2_565
O11 Mo4 O5 73.52(14) . 2_565
O10 Mo4 O2 87.15(16) . 2_565
O9 Mo4 O2 165.02(15) . 2_565
O8 Mo4 O2 84.54(16) . 2_565
O11 Mo4 O2 72.15(14) . 2_565
O5 Mo4 O2 72.48(12) 2_565 2_565
O10 Mo4 Mo1 138.61(14) . 2_565
O9 Mo4 Mo1 85.79(13) . 2_565
O8 Mo4 Mo1 119.17(11) . 2_565
O11 Mo4 Mo1 35.13(10) . 2_565
O5 Mo4 Mo1 41.50(9) 2_565 2_565
O2 Mo4 Mo1 79.34(9) 2_565 2_565
N7 C1 N8 113.9(7) . .
N7 C1 H1 123.0 . .
N8 C1 H1 123.0 . .
N9 C2 N7 113.9(8) . .
N7 C2 N9A 99.9(14) . .
N8 C3 C4 112.5(5) . .
N8 C3 H3A 109.1 . .
C4 C3 H3A 109.1 . .
N8 C3 H3B 109.1 . .
C4 C3 H3B 109.1 . .
H3A C3 H3B 107.8 . .
C6 C4 C5 119.0(5) 2_774 .
C6 C4 C3 120.3(5) 2_774 .
C5 C4 C3 120.7(5) . .
C6 C5 C4 119.9(5) . .
C6 C5 C10 120.6(5) . .
C4 C5 C10 119.5(5) . .
C5 C6 C4 121.1(5) . 2_774
C5 C6 C7 119.6(5) . .
C4 C6 C7 119.3(5) 2_774 .
N5 C7 C6 111.4(4) . .
N5 C7 H7A 109.3 . .
C6 C7 H7A 109.3 . .
N5 C7 H7B 109.3 . .
C6 C7 H7B 109.3 . .
H7A C7 H7B 108.0 . .
N6 C8 N4 114.2(6) . .
N6 C8 H8 122.9 . .
N4 C8 H8 122.9 . .
N4 C9 N5 110.8(6) . .
N4 C9 H9 124.6 . .
N5 C9 H9 124.6 . .
N2 C10 C5 111.5(5) . .
N2 C10 H10A 109.3 . .
C5 C10 H10A 109.3 . .
N2 C10 H10B 109.3 . .
C5 C10 H10B 109.3 . .
H10A C10 H10B 108.0 . .
N1 C11 N2 109.5(5) . .
N1 C11 H11 125.2 . .
N2 C11 H11 125.2 . .
N3 C12 N1 114.6(6) . .
N3 C12 H12 122.7 . .
N1 C12 H12 122.7 . .
C11 N1 C12 104.0(5) . .
C11 N1 Co1 130.2(4) . .
C12 N1 Co1 125.8(4) . .
C11 N2 N3 109.2(5) . .
C11 N2 C10 128.8(5) . .
N3 N2 C10 121.8(4) . .
C12 N3 N2 102.7(5) . .
C9 N4 C8 102.6(5) . .
C9 N4 Co1 134.3(4) . 1_655
C8 N4 Co1 123.0(4) . 1_655
C9 N5 N6 109.3(5) . .
C9 N5 C7 129.2(5) . .
N6 N5 C7 121.4(5) . .
C8 N6 N5 103.1(5) . .
C1 N7 C2 101.6(6) . .
C1 N7 Co1 134.2(5) . 1_565
C2 N7 Co1 123.5(5) . 1_565
C1 N8 N9A 103.5(14) . .
C1 N8 N9 108.3(6) . .
C1 N8 C3 129.9(6) . .
N9A N8 C3 120.9(14) . .
N9 N8 C3 120.3(6) . .
N9A N9 C2 86(2) . .
N9A N9 N8 69(2) . .
C2 N9 N8 101.5(8) . .
N9 N9A N8 71(2) . .
N9 N9A C2 57.3(17) . .
N8 N9A C2 91(2) . .
Mo1 O2 Mo3 110.25(18) 2_565 .
Mo1 O2 Mo4 110.68(15) 2_565 2_565
Mo3 O2 Mo4 104.07(16) . 2_565
Mo1 O5 Mo4 93.18(14) . 2_565
Mo1 O5 Mo1 104.48(15) . 2_565
Mo4 O5 Mo1 97.11(12) 2_565 2_565
Mo1 O5 Mo3 91.44(13) . 2_565
Mo4 O5 Mo3 164.13(18) 2_565 2_565
Mo1 O5 Mo3 96.41(13) 2_565 2_565
Mo1 O5 Mo2 163.61(17) . 2_565
Mo4 O5 Mo2 86.68(12) 2_565 2_565
Mo1 O5 Mo2 91.78(12) 2_565 2_565
Mo3 O5 Mo2 84.63(11) 2_565 2_565
Mo4 O8 Mo2 117.81(19) . .
Mo4 O9 Co1 155.7(2) . 2_665
Mo4 O10 Co1 157.7(2) . .
Mo1 O11 Mo4 109.37(17) 2_565 .
Mo1 O11 Mo3 111.31(17) 2_565 2_565
Mo4 O11 Mo3 103.32(15) . 2_565
Mo1 O12 Mo2 118.48(19) . .
Mo3 O13 Mo2 118.1(2) . .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Co1 N1 2.096(5) .
Co1 N4 2.110(5) 1_455
Co1 O9 2.110(4) 2_665
Co1 N7 2.113(6) 1_545
Co1 O1W 2.117(4) .
Co1 O10 2.159(4) .
Mo1 O4 1.686(4) .
Mo1 O12 1.739(4) .
Mo1 O2 1.950(4) 2_565
Mo1 O11 1.959(3) 2_565
Mo1 O5 2.131(4) .
Mo1 O5 2.386(4) 2_565
Mo1 Mo4 3.2113(7) 2_565
Mo2 O6 1.692(4) .
Mo2 O14 1.704(4) .
Mo2 O13 1.902(4) .
Mo2 O8 1.930(4) .
Mo2 O12 2.290(4) .
Mo2 O5 2.452(4) 2_565
Mo3 O1 1.691(4) .
Mo3 O3 1.694(4) .
Mo3 O13 1.897(4) .
Mo3 O2 2.000(4) .
Mo3 O11 2.344(4) 2_565
Mo3 O5 2.388(3) 2_565
Mo4 O10 1.709(3) .
Mo4 O9 1.717(4) .
Mo4 O8 1.871(4) .
Mo4 O11 1.977(4) .
Mo4 O5 2.287(3) 2_565
Mo4 O2 2.302(4) 2_565
Mo4 Mo1 3.2113(7) 2_565
C1 N7 1.302(8) .
C1 N8 1.310(9) .
C1 H1 0.9300 .
C2 N9 1.335(12) .
C2 N7 1.399(11) .
C2 N9A 1.58(3) .
C3 N8 1.470(8) .
C3 C4 1.502(8) .
C3 H3A 0.9700 .
C3 H3B 0.9700 .
C4 C6 1.399(7) 2_774
C4 C5 1.415(7) .
C5 C6 1.381(8) .
C5 C10 1.518(7) .
C6 C4 1.399(7) 2_774
C6 C7 1.521(7) .
C7 N5 1.471(7) .
C7 H7A 0.9700 .
C7 H7B 0.9700 .
C8 N6 1.305(9) .
C8 N4 1.380(9) .
C8 H8 0.9300 .
C9 N4 1.316(8) .
C9 N5 1.335(8) .
C9 H9 0.9300 .
C10 N2 1.461(7) .
C10 H10A 0.9700 .
C10 H10B 0.9700 .
C11 N1 1.308(7) .
C11 N2 1.345(7) .
C11 H11 0.9300 .
C12 N3 1.308(8) .
C12 N1 1.342(8) .
C12 H12 0.9300 .
N2 N3 1.357(7) .
N4 Co1 2.110(5) 1_655
N5 N6 1.367(7) .
N7 Co1 2.113(6) 1_565
N8 N9A 1.39(3) .
N8 N9 1.406(10) .
N9 N9A 0.96(3) .
O2 Mo1 1.950(4) 2_565
O2 Mo4 2.302(4) 2_565
O5 Mo4 2.287(3) 2_565
O5 Mo1 2.386(4) 2_565
O5 Mo3 2.388(3) 2_565
O5 Mo2 2.452(4) 2_565
O9 Co1 2.110(4) 2_665
O11 Mo1 1.959(3) 2_565
O11 Mo3 2.344(4) 2_565
O4W O4WA 0.95(2) .
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_4
N8 C3 C4 C6 -97.1(6) . 2_774
N8 C3 C4 C5 85.7(6) . .
C6 C4 C5 C6 -1.4(9) 2_774 .
C3 C4 C5 C6 175.9(5) . .
C6 C4 C5 C10 178.8(5) 2_774 .
C3 C4 C5 C10 -4.0(8) . .
C4 C5 C6 C4 1.4(9) . 2_774
C10 C5 C6 C4 -178.8(5) . 2_774
C4 C5 C6 C7 -177.9(5) . .
C10 C5 C6 C7 1.9(8) . .
C5 C6 C7 N5 -96.8(6) . .
C4 C6 C7 N5 83.9(6) 2_774 .
C6 C5 C10 N2 -78.6(7) . .
C4 C5 C10 N2 101.2(6) . .
N2 C11 N1 C12 -0.6(7) . .
N2 C11 N1 Co1 -178.9(4) . .
N3 C12 N1 C11 0.7(9) . .
N3 C12 N1 Co1 179.0(5) . .
N4 Co1 N1 C11 139.9(6) 1_455 .
O9 Co1 N1 C11 -37.8(6) 2_665 .
N7 Co1 N1 C11 -126.1(6) 1_545 .
O1W Co1 N1 C11 48.4(6) . .
N4 Co1 N1 C12 -38.0(6) 1_455 .
O9 Co1 N1 C12 144.4(6) 2_665 .
N7 Co1 N1 C12 56.0(6) 1_545 .
O1W Co1 N1 C12 -129.4(6) . .
N1 C11 N2 N3 0.4(7) . .
N1 C11 N2 C10 175.3(6) . .
C5 C10 N2 C11 158.0(6) . .
C5 C10 N2 N3 -27.7(8) . .
N1 C12 N3 N2 -0.4(9) . .
C11 N2 N3 C12 0.0(8) . .
C10 N2 N3 C12 -175.3(6) . .
N5 C9 N4 C8 -0.3(7) . .
N5 C9 N4 Co1 178.6(4) . 1_655
N6 C8 N4 C9 0.4(8) . .
N6 C8 N4 Co1 -178.6(5) . 1_655
N4 C9 N5 N6 0.0(8) . .
N4 C9 N5 C7 -175.3(5) . .
C6 C7 N5 C9 -151.0(6) . .
C6 C7 N5 N6 34.2(8) . .
N4 C8 N6 N5 -0.4(8) . .
C9 N5 N6 C8 0.2(8) . .
C7 N5 N6 C8 176.0(6) . .
N8 C1 N7 C2 4.2(9) . .
N8 C1 N7 Co1 174.1(5) . 1_565
N9 C2 N7 C1 1.8(11) . .
N9A C2 N7 C1 -34.2(15) . .
N9 C2 N7 Co1 -169.5(6) . 1_565
N9A C2 N7 Co1 154.5(13) . 1_565
N7 C1 N8 N9A 32.9(15) . .
N7 C1 N8 N9 -8.5(9) . .
N7 C1 N8 C3 -174.4(6) . .
C4 C3 N8 C1 -157.2(6) . .
C4 C3 N8 N9A -8.5(17) . .
C4 C3 N8 N9 38.2(8) . .
N7 C2 N9 N9A -74(2) . .
N7 C2 N9 N8 -6.3(11) . .
N9A C2 N9 N8 68(2) . .
C1 N8 N9 N9A 89(2) . .
C3 N8 N9 N9A -103(2) . .
C1 N8 N9 C2 8.5(10) . .
N9A N8 N9 C2 -81(2) . .
C3 N8 N9 C2 176.1(7) . .
C2 N9 N9A N8 104.1(11) . .
N8 N9 N9A C2 -104.1(11) . .
C1 N8 N9A N9 -102.5(18) . .
C3 N8 N9A N9 101.7(18) . .
C1 N8 N9A C2 -47.8(15) . .
N9 N8 N9A C2 54.8(15) . .
C3 N8 N9A C2 156.4(9) . .
N7 C2 N9A N9 116.9(19) . .
N9 C2 N9A N8 -66.5(18) . .
N7 C2 N9A N8 50.4(16) . .
O1 Mo3 O2 Mo1 178.56(19) . 2_565
O3 Mo3 O2 Mo1 70.9(2) . 2_565
O13 Mo3 O2 Mo1 -50.6(4) . 2_565
O11 Mo3 O2 Mo1 -97.01(17) 2_565 2_565
O5 Mo3 O2 Mo1 -21.28(15) 2_565 2_565
O1 Mo3 O2 Mo4 -62.72(19) . 2_565
O3 Mo3 O2 Mo4 -170.42(17) . 2_565
O13 Mo3 O2 Mo4 68.1(3) . 2_565
O11 Mo3 O2 Mo4 21.71(12) 2_565 2_565
O5 Mo3 O2 Mo4 97.44(14) 2_565 2_565
O4 Mo1 O5 Mo4 82.90(17) . 2_565
O12 Mo1 O5 Mo4 -95.7(4) . 2_565
O2 Mo1 O5 Mo4 -177.14(15) 2_565 2_565
O11 Mo1 O5 Mo4 -17.51(14) 2_565 2_565
O5 Mo1 O5 Mo4 -98.18(14) 2_565 2_565
O4 Mo1 O5 Mo1 -178.91(16) . 2_565
O12 Mo1 O5 Mo1 2.4(4) . 2_565
O2 Mo1 O5 Mo1 -78.95(15) 2_565 2_565
O11 Mo1 O5 Mo1 80.67(15) 2_565 2_565
O5 Mo1 O5 Mo1 0.0 2_565 2_565
Mo4 Mo1 O5 Mo1 98.18(14) 2_565 2_565
O4 Mo1 O5 Mo3 -81.91(16) . 2_565
O12 Mo1 O5 Mo3 99.4(4) . 2_565
O2 Mo1 O5 Mo3 18.05(13) 2_565 2_565
O11 Mo1 O5 Mo3 177.67(15) 2_565 2_565
O5 Mo1 O5 Mo3 97.00(15) 2_565 2_565
Mo4 Mo1 O5 Mo3 -164.81(18) 2_565 2_565
O4 Mo1 O5 Mo2 -6.2(6) . 2_565
O12 Mo1 O5 Mo2 175.2(5) . 2_565
O2 Mo1 O5 Mo2 93.8(6) 2_565 2_565
O11 Mo1 O5 Mo2 -106.6(6) 2_565 2_565
O5 Mo1 O5 Mo2 172.8(7) 2_565 2_565
Mo4 Mo1 O5 Mo2 -89.1(6) 2_565 2_565
O10 Mo4 O8 Mo2 179.2(2) . .
O9 Mo4 O8 Mo2 71.6(2) . .
O11 Mo4 O8 Mo2 -50.3(4) . .
O5 Mo4 O8 Mo2 -21.3(2) 2_565 .
O2 Mo4 O8 Mo2 -94.5(2) 2_565 .
Mo1 Mo4 O8 Mo2 -19.9(3) 2_565 .
O6 Mo2 O8 Mo4 -179.4(2) . .
O14 Mo2 O8 Mo4 -72.0(3) . .
O13 Mo2 O8 Mo4 47.2(4) . .
O12 Mo2 O8 Mo4 92.6(2) . .
O5 Mo2 O8 Mo4 20.25(19) 2_565 .
O10 Mo4 O9 Co1 -9.3(6) . 2_665
O8 Mo4 O9 Co1 92.3(6) . 2_665
O11 Mo4 O9 Co1 -115.3(6) . 2_665
O5 Mo4 O9 Co1 170.7(6) 2_565 2_665
O2 Mo4 O9 Co1 -155.8(4) 2_565 2_665
Mo1 Mo4 O9 Co1 -148.8(6) 2_565 2_665
O9 Mo4 O10 Co1 124.8(6) . .
O8 Mo4 O10 Co1 20.6(7) . .
O11 Mo4 O10 Co1 -134.4(6) . .
O5 Mo4 O10 Co1 -55.4(9) 2_565 .
O2 Mo4 O10 Co1 -63.5(6) 2_565 .
Mo1 Mo4 O10 Co1 -133.8(5) 2_565 .
N4 Co1 O10 Mo4 60.3(6) 1_455 .
O9 Co1 O10 Mo4 -121.8(6) 2_665 .
N7 Co1 O10 Mo4 -33.6(7) 1_545 .
O1W Co1 O10 Mo4 151.7(6) . .
O10 Mo4 O11 Mo1 179.37(18) . 2_565
O9 Mo4 O11 Mo1 -73.0(2) . 2_565
O8 Mo4 O11 Mo1 50.1(3) . 2_565
O5 Mo4 O11 Mo1 20.46(15) 2_565 2_565
O2 Mo4 O11 Mo1 96.90(18) 2_565 2_565
O10 Mo4 O11 Mo3 60.75(19) . 2_565
O9 Mo4 O11 Mo3 168.42(16) . 2_565
O8 Mo4 O11 Mo3 -68.6(3) . 2_565
O5 Mo4 O11 Mo3 -98.16(15) 2_565 2_565
O2 Mo4 O11 Mo3 -21.73(12) 2_565 2_565
Mo1 Mo4 O11 Mo3 -118.6(2) 2_565 2_565
O4 Mo1 O12 Mo2 -179.8(2) . .
O2 Mo1 O12 Mo2 76.6(2) 2_565 .
O11 Mo1 O12 Mo2 -75.4(2) 2_565 .
O5 Mo1 O12 Mo2 -1.2(5) . .
O5 Mo1 O12 Mo2 1.25(18) 2_565 .
Mo4 Mo1 O12 Mo2 -73.6(2) 2_565 .
O6 Mo2 O12 Mo1 -179.3(2) . .
O14 Mo2 O12 Mo1 -6.1(7) . .
O13 Mo2 O12 Mo1 77.1(2) . .
O8 Mo2 O12 Mo1 -77.5(2) . .
O5 Mo2 O12 Mo1 -1.28(18) 2_565 .
O1 Mo3 O13 Mo2 -179.1(2) . .
O3 Mo3 O13 Mo2 -70.1(3) . .
O2 Mo3 O13 Mo2 50.2(4) . .
O11 Mo3 O13 Mo2 93.7(2) 2_565 .
O5 Mo3 O13 Mo2 21.6(2) 2_565 .
O6 Mo2 O13 Mo3 179.2(2) . .
O14 Mo2 O13 Mo3 70.9(3) . .
O8 Mo2 O13 Mo3 -47.7(4) . .
O12 Mo2 O13 Mo3 -92.9(2) . .
O5 Mo2 O13 Mo3 -21.2(2) 2_565 .
